Magnesium-Based Sacrificial Anode Cathodic Protection ... · PDF fileMagnesium-Based...
Embed Size (px)
Transcript of Magnesium-Based Sacrificial Anode Cathodic Protection ... · PDF fileMagnesium-Based...
Metals 2012, 2, 353-376; doi:10.3390/met2030353
metals ISSN 2075-4701
Magnesium-Based Sacrificial Anode Cathodic Protection Coatings (Mg-Rich Primers) for Aluminum Alloys
Shashi S. Pathak, Sharathkumar K. Mendon, Michael D. Blanton and James W. Rawlins *
School of Polymers and High Performance Materials, The University of Southern Mississippi, Hattiesburg, MS 39406, USA; E-Mails: email@example.com (S.S.P.); firstname.lastname@example.org (S.K.M.); email@example.com (M.D.B.)
* Author to whom correspondence should be addressed; E-Mail: firstname.lastname@example.org; Tel.: +1-601-266-4781; Fax: +1-601-266-5880.
Received: 31 May 2012; in revised form: 6 August 2012 / Accepted: 21 August 2012 / Published: 14 September 2012
Abstract: Magnesium is electrochemically the most active metal employed in common structural alloys of iron and aluminum. Mg is widely used as a sacrificial anode to provide cathodic protection of underground and undersea metallic structures, ships, submarines, bridges, decks, aircraft and ground transportation systems. Following the same principle of utilizing Mg characteristics in engineering advantages in a decade-long successful R&D effort, Mg powder is now employed in organic coatings (termed as Mg-rich primers) as a sacrificial anode pigment to protect aerospace grade aluminum alloys against corrosion. Mg-rich primers have performed very well on aluminum alloys when compared against the current chromate standard, but the carcinogenic chromate-based coatings/pretreatments are being widely used by the Department of Defense (DoD) to protect its infrastructure and fleets against corrosion damage. Factors such as reactivity of Mg particles in the coating matrix during exposure to aggressive corrosion environments, interaction of atmospheric gases with Mg particles and the impact of Mg dissolution, increases in pH and hydrogen gas liberation at coating-metal interface, and primer adhesion need to be considered for further development of Mg-rich primer technology.
Keywords: magnesium; sacrificial anode; cathodic protection; Mg-rich primers; anticorrosive coatings; aluminum alloys; corrosion protection
Metals 2012, 2
Magnesium is the sixth most abundant element found in the earths crust, occurring in over 80 minerals that contain more than 20% Mg by weight. Carbonates are the most common form of Mg in nature. Magnesite [MgCO3], dolomite [CaCO3MgCO3], brucite [Mg(OH)2], bishovite [MgCl26H2O], carnallite (KClMgCl26H2O) and olivine [(MgFe)2SiO4] have been considered as raw materials for Mg metal production . The other major source of Mg is MgCl2 from seawater.
Mg is the most electrochemically active metal used in engineering applications (Table 1), and corrodes so readily in some environments that Mg and Mg alloys are purposely utilized as sacrificial anodes on steel structures, such as ship hulls and steel pipes. Mg and Mg alloys stored at room temperature (STP) or in humid atmospheric conditions develop a compositionally varied surface film, consisting of Mg oxide, hydroxide, and carbonates. These films are less stable than the passive films formed on metals such as aluminum and stainless steels. The corrosion protection ability of the surface film is highly dependent on environmental conditions, such as humidity, chloride ion concentration, and interaction with atmospheric gases. Corrosion behavior and corrosion protection methods of Mg and its alloys have been reviewed by several researchers . Corrosion resistance of Mg alloys decreases with increasing relative humidity (RH) and decreasing pH (below 11.5). Consistently, Mg resists corrosion in alkaline solutions when the pH value is above 11.5.
Table 1. Property comparison.
Properties of Magnesium Aluminum Iron
Crystal structure Hcp Fcc Bcc Ease of fabrication and joining of Mg
Density at 20 C (g/cc) 1.74 2.70 7.86 Al is ~2.9 and Mg is ~4.5 lighter than Fe
Coefficient of thermal expansion 20100 (106/C) 25.2 23.6 11.7 Elastic modulus (106 psi) 6.4 10 30 Melting point (C) 650 660 1536
Standard reduction potential (V vs. Standard Hydrogen Electrode)
2.37 1.66 0.447 Higher reactivity of Mg and Al with atmosphere than Fe Mg can act as sacrificial anode
Cost Mg > Al > Fe
Mgs high strength to weight ratio, low density (~66% of aluminum and 25% of iron), high specific stiffness, high thermal conductivity and electromagnetic shielding properties make it a popular choice in various lightweight applications in aircrafts, automobiles, electronics, and medical implant components. Although Mg is available commercially with purity above 99.5%, it is rarely used in engineering applications without being alloyed, due to inherent limitations such as low elastic modulus, limited high strength and creep resistance at elevated temperatures, high degree of shrinkage on solidification, high chemical reactivity and limited corrosion resistance. The most commonly used Mg alloys contain Al, Zn, and Mn; Al and Zn are added in ingot form, dissolving readily at normal melt temperature (~700 C). Al, Zn and Mn are the major alloying elements in Mg alloys. Keeping corrosion protection in mind, alloying elements (Al, Zn, Mn) and heavy-metal impurities (Ni, Fe, Cu) of Mg alloys have to
Metals 2012, 2
be controlled according to the endurance limit. Excess addition of Mn enhances the formation of nobler Al Mn (Fe) secondary phase with Al or Fe which is detrimental to the corrosion resistance of Mg alloys. Mg alloys such as AZ91D, AZ91E, and AM60B contain very low levels of the heavy metal impurities and offer far better corrosion resistance than ordinary Mg alloys. The number of applications for Mg alloys is increasing every year, primarily in the automotive and aerospace sectors.
The established corrosion rate of the secondary phases in Mg alloys is very low when the pH is between 4 and 14. Corrosion of Mg alloys in neutral or alkaline salt solutions is usually initiated as pitting at secondary phase particles. The thickness of the oxide film on secondary phases formed in solution (pH 12) was shown to be several times the thickness formed in air and increased with decreasing pH . The type of processing (ingot, die-cast and extruded Mg or its alloys) also influenced the nature and severity of the corrosion process due to subtle but important morphology differences. For instance, the corrosion rate of AZ91 ingot and die-cast was higher in acidic solutions (pH 12) than in neutral and highly alkaline solutions (pH 4.512) . In comparison, extruded Mg alloy AM60 does not exhibit the same phenomenon in 3.5% NaCl solution at different pH values, however, it undergoes severe pitting corrosion at pH 7 in the absence of pitting (except on the edges) at pH 12. With the shift towards higher chloride ion concentration, the open circuit corrosion potentials shift to more negative values and the corrosion rates increase at all pH levels.
Mg possesses a strong thermodynamic driving force for corrosion and its surface film does not present a very protective kinetic barrier to corrosion . Consequently, Mg is unsuitable for use singularly in applications involving humid and aqueous environments with pH < 12. On the contrary, structural metals such as steel and Al are cathodic to (more noble in galvanic series than) Mg. In these cases, the undesirably high electrochemical activity of Mg has been capitalized upon to provide cathodic protection of nobler structural metals/alloys in pipelines, tanks, and marine structures. The premise of cathodic protection is for an electrical circuit to be established as a means to control the corrosion of a structural metal surface by rendering it as the cathode of a galvanic cell. The use of Al, Zn, Mg, and Sn/In to create activated aluminum alloys, as (1) sacrificial anodes and (2) impressed current cathodic protection systems, are established methods to protect steel structures against corrosion [9,10]. Mg and its alloys have been used as sacrificial anodes for several decades in cathodic protection of oil and gas pipelines, oil drilling platforms cables, heat exchangers, aircraft, ships, and bridges. In these applications, Mg acts sacrificially and transfer corrosion activity away from the structural materials to be protected (cathode). The process results in Mg (anode) dissolution over a given period of time. Figure 1 provides the schematic of sacrificial anode and impressed current protection methods of a pipeline.
Metals 2012, 2
Figure 1. Schematic showing cathodic protection methods using sacrificial anode and impressed current.
2. Interaction of Mg and Its Alloys with the Atmosphere
Corrosion behavior of Mg and its alloys in the atmosphere differs considerably from their behavior in solution. For example, in the presence of sodium chloride in humid air, the surface of Mg is rapidly converted and covered by the white, flaky corrosion products of magnesium hydroxide . Chloride ions are known to promote the corrosion of Mg in aqueous solutions . The anodic reaction (Mg dissolution) under a thin electrolyte layer is diminished compared to a bulk electrolyte . Additionally, the main cathodic process in solution is water reduction, while oxygen reduction is the main cathodic reaction during atmospheric corrosion in thin electrolyte layers [14,15]. The overall rate of corrosion and nature of corrosion products are strongly influenced by the RH and chloride ion concentration.
The natural affinity of Mg and magnesium hydroxide for carbon dioxide has been exploited for CO2 sequestration. Studies investigating the effects of CO2 pressure, temperature, and aqueou